Fatigue strength depending on position of cracks for weldments
This is a study of fatigue strength of weld deposits with transverse cracks in plate up to 50 mm thick. It is concerned with the fatigue properties of welds already with transverse cracks. A previous study of transverse crack occurrence, location and microstructure in accordance with welding conditions was published in the Welding Journal (Lee et al., 1998). A fatigue crack develops as a result of stress concentration and extends with each load cycle until fatigue occurs, or until the cyclic loads are transferred to redundant members. The fatigue performance of a member is more dependent on the localized state of stress than the static strength of the base metal or the weld metal. Fatigue specimens were machined to have transverse cracks located on the surface and inside the specimen. Evaluation of fatigue strength depending on location of transverse cracks was then performed. When transverse cracks were propagated in a quarter-or half-circle shape, the specimen broke at low cycle in the presence of a surface crack. However, when the crack was inside the specimen, it propagated in a circular or elliptical shape and the specimen showed high fatigue strength, enough to reach the fatigue limit within tolerance of design stresses.
Key WordsFatigue Strength Transverse Cracks Surface Crack Inside Crack Thick-Plate Weldments
Unable to display preview. Download preview PDF.
- Boiler and Pressure Vessel Code, Section XI, 1995, American Society of Mechanical Engineers, pp. 20–23.Google Scholar
- Dreng, T., Robakowshi and Dreng, and Scierski, J. M., 1987, International Conference on Fatigue of Welded Constructions, England, Welding Institute, pp. 445–456.Google Scholar
- Lee, H. W., Kang, S. W. and Um, D. S., 1998, “A Study on Transverse weld cRacks in Thick Steel Plate with the FCAW Process,”Welding Journal, Vol. 77, No. 12, pp. 503–510.Google Scholar
- Lu, B., Zheng, X. and Li, D., 1993, “Fatigue Crack Initiation and Propagation in Butt-Joint weld of an Ultrahigh-Strength Steel,”Welding Journal, Vol. 72, No. 2, pp. 79–86.Google Scholar
- Structural Welding Code -Steel (ANSI/AWS D1.1-98), American Welding Society, Miami, Fla., pp. 175–180.Google Scholar
- Yurioka, N., 1995, “A Chart Method to Determine Necessary Preheat Temperature in Steel Welding,”Journal of Japan Welding Society, pp. 347–350.Google Scholar